Materials 2017, 10, 1066; doi:10.3390/ma10091066 www.mdpi.com/journal/materials Review
Review on the Antimicrobial Properties of
Ahmed Al-Jumaili 1, Surjith Alancherry 1, Kateryna Bazaka 1,2 and Mohan V. Jacob 1,*
1 Electronics Materials Lab, College of Science and Engineering, James Cook University, Townsville,
QLD 4811, Australia; Ahmed.Aljumaili@my.jcu.edu.au (A.A.-J.); Surjith.Alancherry@my.jcu.edu.au (S.A.); email@example.com (K.B.)
2 School of Chemistry, Physics, Mechanical Engineering, Queensland University of Technology,
Brisbane, QLD 4000, Australia
* Correspondence: Mohan.Jacob@jcu.edu.au; Tel: +61-747-814-379
Received: 2 August 2017; Accepted: 6 September 2017; Published: 11 September 2017
Abstract: Swift developments in nanotechnology have prominently encouraged innovative
discoveries across many fields. Carbon-based nanomaterials have emerged as promising platforms for a broad range of applications due to their unique mechanical, electronic, and biological properties. Carbon nanostructures (CNSs) such as fullerene, carbon nanotubes (CNTs), graphene and diamond-like carbon (DLC) have been demonstrated to have potent broad-spectrum antibacterial activities toward pathogens. In order to ensure the safe and effective integration of these structures as antibacterial agents into biomaterials, the specific mechanisms that govern the antibacterial activity of CNSs need to be understood, yet it is challenging to decouple individual and synergistic contributions of physical, chemical and electrical effects of CNSs on cells. In this article, recent progress in this area is reviewed, with a focus on the interaction between different families of carbon nanostructures and microorganisms to evaluate their bactericidal performance.
Keywords: carbon nanostructures; antimicrobial properties; fullerene; carbon nanotubes; graphene; diamond-like carbon
Nanotechnology is a swiftly rising field that significantly contributes to the present progress in the development of effective biomaterials. In order to keep the growth of advancement at the present pace, innovative nanomaterials with novel and unique properties are required. Among various nanomaterials, carbon nanostructures (CNSs) and their derivatives gained significant attention due to their extraordinary properties and potential to apply them in a vast number of existing and emerging applications [1–4]. Indeed, carbon can bond to itself in a unique architecture to form extremely low-dimension structures, including fullerenes (0D), nanotubes (1D), graphene sheets (2D) and diamond-like carbon (3D), as seen in Figure 1. In general, CNSs are recognized for their excellent electrical conductivity, supreme mechanical strength, high thermal conductivity, extraordinarily high surface area, excellent photoluminescent properties , high transparency and structural stability [6,7]. These unique properties make carbon nanoarchitectures promising for applications stretching from thin film transistors , transparent conducting electrodes , photovoltaics , supercapacitors , to biosensors , drug delivery , tissue engineering  and photothermal therapy .
CNSs offer promising potential to engage with biological molecules . In particular, a number of carbon-based nanomaterials have been found to possess powerful bactericidal properties toward pathogenic microorganisms. The mechanism by which CNSs inactivate bacteria is complex and
target microorganisms, and the characteristics of the environment in which cell-CNS interactions take place .
In principle, the bactericidal action of CNSs typically involves a combination of physical and chemical mechanisms [17–19]. Physically, CNSs may cause considerable structural damage to the cell wall and membrane of the microorganism. Furthermore, carbon nanomaterials such as graphene sheets are capable to biologically isolate cells from their microenvironments, which may eventually lead to cell death . Chemical interaction between CNSs and the microorganism surface may lead to generation of toxic substances, such as reactive oxygen species (ROS), placing the cell under oxidative stress. The interactions between CNSs and cells may cause an electron transfer phenomenon, where electrons are progressively drained from the microbial outer surface, which may cause ROS-independent oxidative stress, leading to the biological death .
Figure 1. Several forms of carbon nanostructures.
This manuscript reports the key advancements in the use of several carbon nanostructures including fullerene, carbon nanotubes (CNTs), graphene and diamond-like carbon (DLC) as antibacterial agents. Also, it will critically focus on the antibacterial mechanisms/performance of CNSs and highlight the influence of various factors (e.g., size, light, modifications) on their toxicological profile toward microorganisms.
2. Antimicrobial Performance of Carbon Nanostructures
Table 1. The antimicrobial performance of several forms of Carbon nanostructures (CNSs).
CNSs Type Synthesis Method Modification/Catalyst Dimensions Concentration Species of Bacteria Antibacterial
Efficacy Antibacterial Mechanism Ref.
C60 Four-step reaction Cyclen-functionalized
fullerene derivative 150 to 320 nm 7.5 μg/mL
E. coli, S. aureus
plays a major role 
C60 - Light (160 J/cm
385–780 nm ) - 100 μM
Increase in membrane
C70 SES Research
2 wt % of
PS-P4VP E. coli ~5 log
C70 and Ag-NPs,
synergistically target bacterial cells that increase photo-generated ROS
d = ~1 nm
l = 1–3 μm 5 μg/mL E. coli 86.8%
Irrecoverable damages to the outer membrane, releasing the intracellular content
SWCNT CO incorporated
d = 0.9 nm
l = 2 μm 5 μg/mL E. coli 80.1%
Cells lost their cellular
MWCNT CVD method - d = 30 nm
l = 70 μm 5 μg/mL E. coli 24.4%
The majority of cells still intact and maintain their outer membrane
SWCNT CO decomposition Poly(lactic-co-glycolic acid)
d = ~1 nm l = 300 nm
CNT/polymer S. epidermidis 98%
Cells loss their viability
and deactivated 
SWCNT NanoLab productions
Functional groups (−OH, −COOH, and
d = ~1.5 nm l = 10 μm
Form aggregates that act like needles surrounding the cells
MWCNT NanoLab productions
Functional groups (−OH, −COOH, and
d = 15–30 nm
l = 1–5 μm 500 μg/mL
Minor - 
Graphene oxide Hummers and
Offeman - 0.525 μm P.aeruginosa 92%
Oxidative stress, ROS generation, and laddering of DNA
Reduce graphene oxide
GO - 3.40 μm 0.1 mg/mL P.aeruginosa 90%
Oxidative stress and ROS generation 
Graphene oxide Modified Hummers’
procedure - 205 nm 100 mg/mL E. coli -
phospholipids from the cell membrane
Graphene low-pressure CVD AgNW/water
electrolysis - - C. albicans 100%
Graphene layer reduces the attachment of microbes
- DC sputtering Polytetrafluoroethylen
e hybrid t = 200 nm -
S. aureus 56% 51%
Reduce biofilm formation and cell attachments 
Multilayer films Pulsed-DC-PECVD Germanium t = 1–2 μm 28.9%
germanium P. aeruginosa 62.6%
Disruption to the outer cell wall and leakage of cellular components.
Multilayer films Pulsed-DC-PECVD Germanium t = 1–2 μm 28.9%
germanium S. aureus - Minor reduction in biofilm  Two layers
(a-SiC:H/F-DLC) RF-PECVD Fluorine t = 1 μm 6.5–39.2 at % F P. fluorescens 48.8%
Reduce bacterial attachment and proliferation.
* Diamond has carbon atoms in sp3 hybridization arranged in a face-centered cubic crystal, while graphite has sp2 hybridization structured in a hexagonal close-packed
crystal. DLC is a combination of sp2 and sp3, and the differences in the diamond/graphite arrangements and their chemical bonds cause high variation in DLC properties,
There are many published reports that demonstrate biological activity of fullerene-caged particles [31,43,44]. Several mechanisms have been proposed to describe the bactericidal action of fullerene materials.
In particular, fullerenes and their derivatives have demonstrated powerful antibacterial activity against a wide spectrum of microorganisms when exposed to light [29,30]. One possible explanation for this bactericidal behavior is related to the unique structure of the fullerene particle. From structural design point of view, fullerene is a closed-cage nanoparticle, where the conjugation is
extended through π-electrons. This structure is perhaps the main reason that fullerenes can absorb
light and subsequently generate reactive oxygen species . As soon as fullerene (C60) is illuminated
by photons, C60 will excite from the ground state to an extremely short-lived (~1.3 ns) excited state.
The excited state quickly decays to a lower triplet state that has a longer lifetime (50–100 μs) .
Then, in presence of molecular oxygen (3O2), fullerene may produce ROS, including singlet oxygen
(1O2), through energy transfer photochemical pathway and superoxide anion (O2−) through electron
transfer pathway, as illustrated in Figure 2A . These radicals are short-lived oxidants containing one or more unpaired electrons excited in their highest occupied atomic/molecular level [47,48]. ROS are generally accepted to be responsible for eukaryotic lipid peroxidation and eukaryotic cell membrane interruption [29,49–51]. High level of ROS is acutely lethal to microorganisms , triggering damage to cellular molecules like lipids, proteins, and nucleic acids . Interestingly, in some cases, fullerenes particles in dark sites may act as antioxidants, avoiding lipid peroxidation induced by hydroxyl and superoxide radicals .
The physical interaction between fullerenes and the outer microbial membrane is another antibacterial mechanism, where fullerene NPs induce cell membrane disruption and/or DNA cleavage due to high surface hydrophobicity of the particle, which can easily interact with membrane lipids . As different bacterial species have dissimilar cell wall components, this may account for dissimilar fullerene–cell interactions. Generally, fullerene particles are found to be more biologically-active toward gram positive bacterial species rather than gram negative microorganisms, suggesting that the bactericidal success is reliant on the fullerene insertion into the bacterial cell wall . Experimental data have shown that P. putida diminished its levels of unsaturated fatty acids and increased the proportions of cyclopropane fatty acids due to fullerene exposure. This suggests that deterioration of the microorganism related to cell wall damage, namely alterations in membrane lipid structure and membrane permeability, may be an important aspect of fullerene bioactivity .
From physical point of view, electrostatic forces between fullerenes and a bacterial surface play an important role during their interactions. In order to study electrostatic relations of fullerenes, effects of four forms of fullerene compounds (C60, C60−OH, C60−COOH and C60−NH2) on E. coli and S.
oneidensis were investigated. The positively charged C60−NH2, at concentrations as low as 10 mg/L,
had an acute effect on cellular integrity as seen in Figure 2B,C, and reduced substrate uptake for both
microorganisms . Neutrally charged (C60 and C60−OH) had mild antibacterial influence on S.
oneidensis, while the negatively charged C60−COOH did not impact the growth of either
microorganism. This finding shows that the interaction of positively charged fullerenes with the negatively charged bacterial membranes is more effective than that of neutral and negatively charged fullerene particles . In the same way, several researchers observed the electrostatic attraction to play a major role in the cytotoxic action of fullerene derivatives, causing membrane stress mediated by direct physical contacts, while the role of oxidative stress was considered minor.
The bacterial respiratory chain (located in the membrane) can be also affected by fullerene particles, signifying one further bacteriostatic mechanism . It is quite possible that fullerene nanoparticles interfere with the cellular energy metabolism chain as opposed to physically disrupting the bacterial membrane. The high concentrations of fullerene derivatives possibly increase the uptake of O2, triggering an increase in its conversion to H2O2, which in turn interferes with the respiratory
Figure 2. (A) Schematic representation of fullerene C60 photochemical pathways leading to reactive oxygen species (ROS) generation. Reprinted with permission from Reference ; (B,C) SEM images of S. oneidensis MR-1 cells treated with C60−NH2 show cellular damage. Cell samples were fixed for SEM images approximately 1 h after exposure to 20 mg/L C60−NH2. Green arrow points to nanoparticle aggregations and red arrow points to the damaged part of the cell. Reprinted with permission from Reference .
Theoretical approaches (simulations) have also been used to predict the mechanisms by which
fullerenes penetrate microbial membranes. Molecular dynamic simulations showed that C60
translocation is highly dependent on the specific lipid structures of the target pathogen. C60 has a
limited tendency to enter homogeneous bilayers of incomplete core lipopolysaccharides, but the
translocation of C60 into bilayers of complete core lipopolysaccharide is not a thermodynamically
favored process. The same simulation revealed that small changes in temperature, ambient ion concentrations, lipopolysaccharide core sugar length, or the incidence of phospholipid defects result
in large differences in the interactions between the C60 and the surface membranes . It is important
to note that the bio-reactivity of nanomaterials toward biological targets not only depends on the cell wall structure but also is subject to cellular enzymes and metabolic activities of the microorganism . Bearing in mind the influence of ambient conditions and microorganism cellular activities will help to understand the inconsistent toxicological results observed in aforementioned fullerene studies.
Various types of functionalization are being subjugated to fullerene compounds with the aim to control their interactions with biological molecules. The combination of the carboxy-functionalized fullerene into the microbial wall was identified, proposing that the antibacterial performance initiated through its insertion into the cell wall and damaging followed to the membrane’s integrity . In
order to study antimicrobial activity of fullerene with different functionalities, two C70-derivatives
were fabricated , namely one with a decacationic side chain (LC17) and another with the same decacationic side chain plus an extra deca-tertiary-amine side chain (LC18) . The
eradicating six logs of both gram-positive and gram-negative microorganisms. Interestingly, the attachment of an additional arm allowed the moiety to act as an effective electron donor and improved the generation yield of hydroxyl radicals under UVA illumination. The white light was more bio-active with LC17, whereas UVA light was more bio-active with LC18 .
Modification of cationic C60 with iodide could create powerful bactericidal fullerene. The
antimicrobial mechanism of cationic C60/iodide may involve photo-induced electron reduction of
1(C60>)* or 3(C60>)* by iodide generating I or I2, followed by successive intermolecular electron-transfer
actions of (C600>)− to yield reactive radicals . It is worth mentioning the ability of fullerene
materials to generate ROS is strongly influenced by chemical modification of the cage . For
example, the rate of ROS (singlet-oxygen) production is slower for functionalized C80 than for the
un-functionalized fullerenes . Often, chemical fictionalization of fullerene particles reduces bond
angles from 120° in sp2 down to 109.5° in sp3, rendering the modified molecule more stable .
Fullerenes are highly insoluble in water, however uniformly-distributed aqueous suspension
can be prepared using fullerene derivatives . Fullerene suspensions (e.g., aggregations of C60) are
identified to possess biological activities against microorganisms, possibly distinct from those of bulk solid fullerene . In aquatic systems, it has been argued that the fullerene particles will not necessarily puncture the microbial cell nor generate ROS, but instead exert toxicity as a particle via chemical interactions upon direct contact [68,69]. In this regard, it demonstrated that fullerene
aqueous solution is an efficient photo-induced antibacterial agent, even at low concentration (C60 =
1.8 × 10−2 mM) able to effectively suppress the growth of gram-positive microorganisms . C70
suspension is demonstrated to be more photoactive than nC60 (forming more 1O2 than nC60 for
wavelengths 300–650 nm) resulting in a consistent ratio of 1.69 ± 0.05 times the 1O2 creation of nC60
. Similarly, suspension of C60/pyrrolidinium is an extremely active broad-spectrum bactericidal
photosensitizer, capable to eradicate more than 99.99% of bacterial and fungal cells in vitro once irradiate with white light . Moreover, the irradiation of dissolved polyhydroxylated fullerene (fullerol) by UV radiation (310 to 400 nm) significantly increased the inactivation of bacteriophage MS2 (up to 4 log) due to ROS generation. In the absence of UV, fullerol revealed limited biological activity due to negligible ROS production . However, generally, one shortcoming of soluble functionalized fullerenes is lying in their absorption range, which is inclined toward the blue and green visible spectrum rather than the red/far red band that have better tissue penetration .
Likewise, unmodified fullerenes such as C60 have high hydrophobicity and innate tendency to
aggregate, preventing efficient photo-activity . It is important to mention that the antibacterial performance of fullerene suspensions is also influenced by the preparation methods used. For example, aqueous fullerene suspensions were prepared using four different procedures, namely
using tetrahydrofuran (THF) as a solvent (THF/nC60), sonicating C60 dissolved in toluene with water
(son/nC60), stirring C60 powder in water (aq/nC60), and using a solubilizing agent (PVP/C60). All four
fullerene derivatives revealed antibacterial activity toward B. subtilis, where THF/nC60 appeared to
have a more effective antimicrobial outcome than the other preparations due to variability in the extraction method .
To summarize the fullerene antibacterial activities:
• Fullerene is capable of inducing cell membrane disruption and/or DNA cleavage in
• Fullerenes can inactivate microorganisms by impacting their cellular energy metabolism chain.
• Upon light illumination, fullerenes generally yield high rate of ROS that increase the
3.1. Carbon Nanotubes (CNTs)
In 2007, Kang et al. reported the first article presenting strong antimicrobial performance of single wall carbon nanotubes (SWCNTs) against E. coli pathogen . Later, numerous studies proved that
both SWCNTs and multi-wall carbon nanotubes (MWCNTs) have powerful inhibitory effects against
have demonstrated significantly higher antibacterial performance in comparison with MWCNTs
(and even fullerene-C60) . Despite the incredible material properties and vast number of reports
on their antibacterial effects, the bactericidal mechanism of CNTs are yet to be fully understood. The mechanism of carbon nanotube toxicity is highly influenced by several factors such as diameter, length, residual catalyst, electronic structure, surface functional group, surface chemistry and coatings of the CNT . In particular, the length of nanotubes is crucially important during interactions with the cell membrane. The shorter tube is founded to exert higher bactericidal performance in comparison to longer tubes . The shorter length may increase the chances for interaction between open ends of nanotubes and a microorganism, leading to extra cell membrane
damage . Interestingly, it was observed that when the length of MWCNTs reach up to 50 μm, the
tube wrapped around the surface of microbial cell and consequently promoted osmotic lysis of the microorganism . Unlike the solid surface, the interaction of CNTs with cells in a liquid medium is quite different. Longer nanotubes have exhibited higher antibacterial performance than shorter ones. In a liquid system, the short length of CNTs are more likely to self-aggregate without involving a large number of microbial cells, while longer nanotube aggregates are more bio-effective as they affect a larger number of cells in the aggregates . It is well known that aggregation/agglomeration of CNTs is inevitable owing to their unique configuration and powerful van der Waals interactions [83,84].
The diameter of a tube also plays a significant role in the bacterial inactivation process. Smaller diameters can promote damage to cell membrane through the cell-surface interaction [85,86]. Direct microscopic observations have shown that individual CNTs (small diameter ~1.5 nm) attached at one end to the microorganism, protruding from the cell surface with the other end much like ‘needles’ of the hedgehog. Furthermore, the small tubes made the bacteria interact closely with each other. CNTs with large diameter (~15–30 nm) mostly interact with bacteria by their side walls, where the cells were just located on top of the carbon tubes instead of tightly interacting with CNTs bunches . Due to nature of the shape, CNTs maybe have less bactericidal action toward rod-shaped bacteria when compared to spherical ones .
Another important factor affecting the antimicrobial efficacy of CNTs is emanated from their electronic structure. As known, several parameters (e.g., tube diameter, orientation of the tubes and wrapping angle) highly influence the electronic conductivity of SWCNTs, and small differences in these features could shift the tubes from a metallic to semiconducting state [87,88]. Interestingly, reports have revealed that electronic structure is a significant element governing the antimicrobial action of SWCNTs. The loss of bacterial viability was observed to be positively related to the ratio of metal SWCNTs in samples of similar length, diameter, and number of defect spots .
CNTs are well known to possess excellent electrical conductors with high dielectric breakdown strength and possess outstanding field electron emission properties . Employing CNTs as a discharge electrode in the corona plasma system may significantly reduce the threshold voltage of plasma field. Hence, the CNT-corona discharge system can produce a low operating voltage and yield a low ozone concentration, which can be used to eradicate bioaerosols. The corona discharge
system employing CNTs was reported to inactivate 97% of E. coli bioaerosol cells at discharge
voltages of −7.5 kV, that is significantly higher than using stainless steel electrodes (the inactivation efficiency is 34% at the same voltages) . The electrode behavior can be expanded further by integrating CNSs with several dielectric polymers such as polydimethylsiloxane (PDMA) and polyvinylidene fluoride (PVDF) fibers, which can be used for several applications (e.g., nanoscale aerosol filters, biomedical implants, artificial muscles and robots, sensors) [92,93].
interaction of CNTs with biofilm is highly dependent on the stage of biofilm formation, where the efficacy of CNTs is more pronounced at the early steps of biofilm formation . As soon as microorganisms become protected within the structure of the mature biofilm, they are less susceptible to the influence of CNTs than bacteria in other biofilm phases .
Figure 3. Scanning Electron Microscope (SEM), Confocal Scanning Laser Microscopy (CLSM) and surface plots of biofilm formation of K. oxytoca (a); P. aeruginosa (b) and S. epidermidis (c) on multi-wall carbon nanotubes(MWCNT) (tube length 540 μm) and glass control. Reprinted with permission from Reference .
arrays of pristine CNTs demonstrated strong repression toward biofilms initiated by B. subtilis (biofilm coverage only 6.18% from the substrate), with only individual microcolonies able to form on the surface. These arrays are consisting of tubes much smaller than the usual size of the bacterial cell
(~2 μm), which prevents the penetration of microorganisms in between the nanotubes .
Interestingly, CNTs are capable to significantly impact biofilms in liquid system. CNTs inhibit
microbial biofilms in a concentration dependent mode: 50 μg mL−1 SWCNTs reduction the biofilm by
81.19%, and ≥200 μg mL−1 SWCNTs totally inhibit the biofilm . However, more in-depth
understanding of how CNTs interact with biofilms is needed to engineer appropriate nanomaterial agents to effectively disturb microorganisms at any growth phase or biofilm stage.
In order to evaluate the photo-activities, three carbon nanostructures (fullerene C60, SWCNTs
and MWCNT) were tested for ROS production under UV irradiation. For similar carbon concentrations, SWCNTs exhibited the highest ROS generation followed by MWCNT, and fullerene . Thus far, several attempts have been made to improve the photo-activity of CNTs through the
engagement with various metallic elements. It has been reported that the TiO2/MWNTs/Si surface
(annealed at 400 °C) displayed great photo-catalyst activities and killed virtually all E. coli cells upon contact (in 60 min under the visible light illumination). The Ti–C and Ti–O–C carbonaceous bonds,
created at the TiO2/CNTs interface, become active upon visible light absorption, and efficiently
contributed to the charge transfer between the photo-excited CNTs and the TiO2 film, accordingly
increasing the rate of generation of OH radicals . Furthermore, branched CNTs were prepared
to develop tree-like nanocomposites of TiO2/branched-CNTs, which revealed highly enhanced
photo-catalytic behaviour against C. albicans in comparison with the TiO2/CNTs and TiO2 thin film. The
outstanding visible light-induced biological efficacy of TiO2/branched-CNTs is related to the creation
of electron—hole pairs by light irradiation with a low recombination rate, as well as the high surface area available for the heterostructure–cell interactions .
However, in some cases, the presence of metal particles on bioactive CNTs may negatively affect their antibacterial performance. For example, vertically aligned-MWCNTs arrays were deposited in tip-growth method on Ni/Si substrates using PECVD. The results showed that the Ni-removed Ag– CNTs exhibited a powerful bactericidal performance in the dark (inactivation of ~93% in 60 min), whereas a partial antibacterial activity was observed on the films of Ni-removed CNTs and the Ag– Ni/CNTs (inactivation of ~42% and 31% in 60 min). The Ni seeds performed as obstacles preventing active cell membrane rupture during contact between the microorganisms and the tips of the CNT structures .
It is worth mentioning that collection of CNSs-microscopic data (e.g., SEM and TEM images) requires irradiation of the sample with highly energized electron beams that potentially cause severe catastrophic damages/changes to the structure of CNSs. These damages include heating, electrostatic charging, ionization, displacement damage and sputtering . Crespi et al. reported several high-resolution of CNTs showing anisotropic collapse of the nanotube during microscopy images . Thus, several advanced techniques such as spherical aberration corrected electron microscopy have been developed in order to reduce beam damages in samples, which improved, larger and faster direct-detection electron-counting for images. Also, the aberration correction was found to be very effective to produce two dimensional images to probe the sub-atomic level details of the samples .
functionalized tube . In this regard, the presence of the amino side group on CNTs increases the positively cationic nature of the structure, which leads to an increase in the efficacy of interactions between the nanotubes and the negatively charged microbial walls . It is important to mention that the functionalization/chemical modification of carbon tubes is fundamentally different for both carbon tube types. In the case of SWNT (a one-atom-thick layer), covalent functionalization will break several carbon double bonds (C=C), leaving vacancies/holes in the nanotube’s configuration and thus varying physical and chemical properties. In the case of MWNT, only the outer wall will be structurally modified . For example, studies showed that SWCNTs with surface functionalities
of −OH and −COOH displayed extremely strong bactericidal activity toward both gram-positive and
gram-negative bacteria (in DI water and 0.9% NaCl solution), while MWCNTs with similar functionalities did not display antimicrobial action to either type of microbial cells .
Introducing small quantities of CNTs into a polymer network can also result in a significant increase in the antibacterial performance of that polymer. Remarkably, polymer with only 3% of SWNTs (0.03 mg/mL of SWNT) demonstrated similar or stronger bactericidal performance than the surfaces consisting of 100% SWNTs . Correspondingly, introducing SWCNTs (diameter 0.8 to 1.2 nm) into a biomedical polymer, e.g., poly (lactic-co-glycolic acid), notably increased the antimicrobial activity of the polymer, with ~98% of bacterial cell dying within one hour of exposure . Similarly, combining SWCNTs with polyvinylpyrrolidone–iodine, a medical polymer, created a porous thin coating, where nanotubes are covered with a monolayer polymer. In these coatings, iodine is attached covalently to the external surface of the porous matrix, promoting it to be gradually released into the system and extend the duration of antibacterial events .
From the literature, the main antibacterial mechanisms of CNTs can be summarized to include:
• Disruption of membrane integrity by powerful electrostatic forces between microbial outer
surface and CNTs, leading to oxidation of the membrane.
• Reactive oxygen species generation may directly harm biological molecules of bacteria and/or
indirectly prompt DNA destruction.
• Impurity components (e.g., metallic nanoparticles, catalysts, suspension) that are introduced
into CNT-structures during fabrication processes can contribute in their antibacterial activities [80,82,115].
• It is rationally possible to expect that some of antibacterial mechanisms associated with C60 can
be applicable to SWCNT, in particular the bactericidal oxidative stress, since they are both are made of pure carbon and have similar diameters .
Graphene-related families including pristine graphene (pG), graphene nanosheets (GNS), graphite (Gt), multilayer graphene (MLG), graphene oxide (GO) and reduced graphene oxide (RGO) have been widely explored. In general, it was found that under similar conditions, GO shows the highest antibacterial activity toward P. aeruginosa, followed by rGO, Gt, and GtO . Still, the diverse intrinsic properties of graphene materials (e.g., sheet sizes, layer number, nanopores, shapes, presence of oxygen groups, defect density, quality of the individual graphene sheets, corrugation, hydrophilicity, etc.) make it challenging to predict their exact antimicrobial mechanisms . In order to understand how these nanomaterials interact with microorganisms, several scenarios have been examined.
phospholipid molecules from the lipid layers of the membranes. The extraction of phospholipids causes a sparser lipid bilayer and a distortion of the membrane due to powerful dragging forces from the graphene sheet, consequently resulting in irreversible damage to living systems [37,119]. Figure 4 shows simulations of the interactions between graphene nanosheet and bacterial surfaces.
The physical size, in particular the length and surface area, of graphene nanosheets play a substantial role in their antibacterial activity. A simulation showed that a small graphene sheet (~5.9
× 6.2 nm2) is likely to slowly diffuse through the phospholipid bilayer membrane . Small
nanosheets can enter the membrane without disturbing the order of the phospholipid molecules, while larger sheets (~11 nm) strongly affect the order, the density and the distribution of the phospholipids . On the other hand, interestingly, it has been suggested that direct contact with graphene edges is not an important part of the mechanism. Instead, the availability of the basal planes of GO nanosheets governs whether it is biologically active toward microorganisms or not [122,123]. It is worth mentioning that once graphene sheets are on/within a bacterium, a near-IR light irradiation could kill the cell by immoderate local heating since graphenes can absorb the near-IR irradiation unlike bacteria, which are transparent in this spectroscopic range [124,125].
The oxidative stress mechanism has been proposed as a main cytotoxicity mechanism of graphene . The oxidative stress is often mediated by graphene-based materials through the ROS generation. The over-production of ROS can cause cells to enter a state of oxidative stress that results in extensive damage to cellular components, such as lipids and proteins . The oxidative stress is a key process for bactericidal activity of GO through superoxide anion formation, which leads to the permanent DNA laddering that potentially can kill the cell . Importantly, defect densities on graphene sheet surfaces could also contribute to oxidative stress-related antibacterial events by increasing oxygen adsorption at the defect locations . In this regard, the AFM-based force spectroscopy technique was utilized to point out that GO/bacteria interactions are predominantly repulsive due to lipopolysaccharide bridging, clearly emphasizing the role of oxidative pathways in graphene antibacterial mechanisms .
Nevertheless, additional reports have highlighted that oxidative stress can be triggered without ROS generation, by means of graphene interference with a specific bacterial process through oxidization and disruption of vital biological structures . It was found that reduced graphene nanowalls (RGNWs) revealed higher antibacterial activity compared to unreduced graphene oxide nanowalls (GONWs). The antibacterial action was explained by the presence of sharper edges in RGNWs, which serve as good electron acceptors and promote more powerful interactions with cell membranes and/or enhanced charge transfer between the bacterial surface and the reduced nanowalls . In order to shed more light on the role of electron transfer phenomenon, three types of monolayer graphene on different substrates (conductor (Cu), semiconductor (Ge) and insulator
(SiO2)) were investigated against both gram-negative and gram-positive bacteria. The graphene
layers on Cu and Ge can remarkably impede the growth of both bacteria, while graphene on SiO2 did
not show significant influence toward both species. The powerful antibacterial performance of graphene on Cu and Ge can be attributed to the electron transfer. In this case, graphene/substrate junction performs as an electron pump, where electrons are progressively pumped away from the microbial membrane. The electron transfer can cause a ROS-independent oxidative stress in the affected microorganisms .
Due to its unique dimensional properties, the aggregated graphene sheets in suspensions can trap and isolate bacterial cells from their microenvironment. This physical disconnection from their immediate surrounding will prevent vital glucose consumption and lead to inactivation of bacteria, reducing its ability to proliferate . It has been reported that the antibacterial action of GO sheets
against E. coli is lateral size dependent, by way of larger nanosheet displaying higher bactericidal
performance than smaller ones. Large nanosheets more easily cover the bacterial cells, where cells cannot grow once are fully covered. On the other hand, small sheets may attach to the microbial surface, but cannot fully isolate the cells from their microenvironment, as seen in Figure 4 (N and O) .
lipopolysaccharides, enhancing the attachment of the nanosheets to the bacteria . However, presence of positively charged nanoparticles on the surface of graphene materials will substantially decrease the negative charge of the resultant nanocomposites (nanoparticles/GO). Due to its positive charge and broad-spectrum bactericidal activity toward numerous pathogenic bacteria, silver nanoparticles are preferred for combination with graphene materials. The Ag/graphene nanocomposite has potential to reduce the surface charge, increase the photo-activity, and synergistic antibacterial properties of individual graphene nanosheets. The GO/Ag was reported to have significant antibacterial activity when compared to individual GO and Ag . The composites of rGO–Au were also confirmed to have a potent bactericidal performance, at ~100% killing efficacy toward both gram-positive and gram-negative microorganisms . More recently, large-area graphene monolayer wrapped silver nanowires were syntheses using CVD. Remarkably, the graphene coverage did not decrease the antimicrobial influences of underlying AgNWs. Quite the opposite, the graphene treatment provided considerable advantages, maintaining robust antibacterial performance under tough environmental conditions and showing up to 100% microbial reduction through the electrolysis of water . Similarly, a sandwich-like nanomaterial based on Ag/halloysite nanotubes/rGO showed greater bacteriostasis facility (~100% against both E. coli and S. aureus) compared with individual Ag nanoparticles, rGO nanosheets or their composites. This phenomenon may relate to the synergistic antimicrobial activity of Ag and rGO . Nevertheless, introducing Ag NPs into graphenes may increase the antibacterial activity of the nanoparticles. For example, the combination of Ag and rGO in a hybrid nanomaterial deliver a negatively charged surface for Ag particles, leading to minimal agglomeration of the Ag nanoparticles. The graphene nanosheets served as a delivery system, adhering to the bacteria and increasing the contact between the Ag and the microbial surface . Furthermore, introducing nanoparticles such as iron oxide into graphene-related materials rendered them superparamagnetic, which is a valuable attribute for drug delivery systems .
The large surface area and the incidence of active groups (e.g., hydroxyl and carboxylic) of GO nanosheets have encouraged researchers to explore its surface functionalization procedures. In a recent report, GO samples were synthesized with different levels of oxidation, hydroxyl, and carbon
radical (•C). The GO with the highest level of •C exhibited the most powerful bactericidal properties
through membrane binding and lipid peroxidation. The bactericidal mechanism of GO/•C can be
explained by a three-step process: (i) electron transfer from the •C to one of the C atoms adjacent to
C=C in the lipid; (ii) subsequently electron transfer from this particular C atom to adjoining molecular dioxygen, creating a lipid peroxide radical involving the attached –O–O bond; and (iii) formation of a lipid peroxide from the lipid peroxide radical . Furthermore, GO nanosheets were modified with hyperbranched polyethylenimine, showing good antifouling and antibacterial effects. Treatment with this hybrid material resulted in a significant reduction in the number of microcolonies of E. coli (up to 75%), loss of cellular integrity of bacterial cell membranes and release of cytoplasm .
Several studies have been carried out in order to introduce graphene-related materials into polymer films. Interestingly, only 3 wt % of GO in a poly(N-vinylcarbazole) polymer was able to escalate bactericidal properties up to 30% when used against planktonic cells, and 57% when applied to biofilms, higher than that for untreated GO . More recently, grafting of graphene oxide onto commercial polyamide membranes has been done to promote their antifouling and anti-adhesion properties. The modified membrane revealed a 17-fold decrease in biofouling of E. coli (within 24 h) compared to the unmodified counterpart . Likewise, methanol-derived graphene nanosheets loaded with gentamicin revealed a diffusion dominated release mechanism that caused loss of viability in bacteria .
the Shewanella family, which is capable to reduce GO into graphene under ambient conditions with no inhibition of bacterial growth . In some cases, E. coli bacteria attached to GO films were able to grow faster and develop denser biofilms than cultures without graphenes, suggesting that GO not only lacks bactericidal activities, but that it basically enhanced bacterial proliferation . In the context of these contradictory results regarding the antibacterial efficacy of graphene-based materials, it is difficult to compare the current data. In fact, new systematic experiments are required to estimate the antimicrobial activities of graphene-related families.
In summary, the antibacterial mechanisms of graphene-related materials are:
• Serve cutting/damaging to the cell membrane.
• Destructive extraction of phospholipids from lipid membranes.
• Oxidative stress through ROS generation.
• Oxidative stress independent-ROS generation by charge transfer phenomena.
• Separating microorganisms from their microenvironment.
3.3. Diamond-Like Carbon (DLC)
Diamond-like carbon structures have been explored extensively for their role as excellent protective coatings in bio-applications. DLC films reveal antibiofouling and antibacterial activities
towards microorganisms such as S. epidermidis, S. aureus and P. aeruginosa in vitro [39,146]. The
bacterial adhesion on the DLC is relatively related to their sp2 and sp3 hybridization, and by
decreasing sp3/sp2 ratio, the antibacterial performance is noticeably enhanced . Usually, DLC
comprising high fraction (>80%) of sp3 bonds is preferred for biomaterial coatings due to its good
interaction with human cells and greater wear and corrosion resistance . In order to interpret the bactericidal performance of DLC, several mechanisms have been proposed. One mechanism could be related to the direct physical damages to microorganisms during contact with pure DLC, causing intense membrane impairment and a release of microbial intracellular metabolites . Other researchers suggested that the antimicrobial activity of DLC comes from their chemical inertness due to weakening of the chemical interface in bacterial adhesion process . In many cases, the mechanism of DLC films can be varied based on the microbial species. For example, DLC and DLC/germanium-doped coatings exhibited significant antibiofouling effect against gram-negative bacteria (~90% reduction in biomass), yet did not significantly inhibit gram-positive bacteria . It is worth to mention that there is contrary evidence that show that DLC surfaces have very weak or non-existent antibacterial activities [151–153].
The bactericidal efficacy of DLC films is critically associated with their surface profile, including high smoothness, high dispersive component of the surface energy and hydrophobicity . In particular, strong hydrophobicity of DLC may cause variations of the bacterial cell membrane and lead to the biological death . Further, the surface free energy is a significant factor controlling DLC antibacterial performance. Often, the surface energy value of DLC films is carefully chosen for specific applications. In order to change the value of surface energy, several elements can be introduced to DLC films. For example, addition of fluorine groups produces bonding modifications
by decrease of C–CF bonds and increasing CF and CF2 bonds in DLC, enhancing the films’
antibacterial efficacy due to the increase of the work of adhesion of the films for bacteria . The incidence of fluorine can change the wettability of DLC by decreasing the surface free energy and increasing the contact angle . It is well-known that the initial attachment of microorganisms (e.g., P. fluorescens) is highly associated with the total surface energy, as the number of adhered cells is reduced with decreasing the total surface energy of the films . Thus, considering surface parameters of DLC will be helpful to design bactericidal coatings, through optimisation of the surface energy.
Inorganic nanoparticles are often incorporated in order to trigger/enhance antibacterial properties of DLC. In theory, introducing a metal particle can acts as a catalyst for the foundation of
sp2-rich boundary sites in DLC structure [158,159]. It has been observed that low concentration of Ag
may reduce the amount of carbon atoms bonded in sp2 configuration that promote sp3 bonding,
nanoparticles are well known to enhance the bactericidal activity of DLC. Experimental data indicated that the antimicrobial activity of a-C:H can be significantly increased up to 99.9% once the copper is incorporated (larger than 58.76 wt %) . Further, copper has potential to change the wetting properties of the DLC, which importantly influences the degree of bacterial adhesion. For example, pure DLC surfaces have water contact angle of around 66.8°, but when the Cu concentration increased from 0.1 to 7.0 at %, the contact angle increased from 76.6 to 82.7°. Once the Cu concentration reached 24.4 at %, the contact angle enlarged significantly up to 104.4° . DLC films with hydrophobic properties may increase the bactericidal performance . In some cases, metallic nanoparticles maybe have drawbacks to the DLC matrix. For example, adding silver increased the hydrophobic and antimicrobial outcomes of a-C:H materials, but is accompanied with the shortcoming of lower hardness. Further increases in silver content did not positively contribute to the enhancement of antimicrobial efficacy, yet caused considerable reduction of surface hardness and flatness . It is not yet understood whether the mechanism of NPs embedded within DLC materials is similar to that of free particles, or whether these particles are acting in a different way . Still, DLC/composite films are engaged successfully as engineered antibacterial coatings due to their ability to govern the release of antibacterial nanoparticles .
The surface chemistry of DLC coatings can be controlled by integrating selective dopants (e.g., F, N, Si, B) that enhance a specific property (e.g., bioactivity, corrosion) [165–167]. Remarkably, dopants give a possibility to manufacture coatings that have high antibacterial activity and favorable interaction with human cells. DLC coatings contain both Ag and Si (1.65 at % Si and 2.09 at % Ag) are biocompatible and capable to reduce the viability of the adhered bacteria up to 50%, while the non-doped DLC films have no bactericidal effect . Similarly, the existence of nitrogen in DLC films may enhance the antibacterial performance. It was found that higher nitrogen content in DLC coatings is associated with lower numbers of bacterial cells attached to the surface . Boron element also notably changes surface characteristics of DLC. Boron creates B-rich carbide bonds in
DLC films that increase the sp3/sp2 ratio and decrease surface roughness parameter . The high
sp3 level and low surface roughness typically improve the antibacterial performance of DLC. On the
other hand, some dopants may change the surface chemistry and reduce the bactericidal performance of DLC. For example, high content of silicon can minimize the antibacterial efficacy of the films . Above mentioned studies clearly indicate that dopants have major influence on the surface chemistry and bioactivity of DLC.
In recent years, there has been an increasing interest in the use of environmentally friendly approaches to develop DLC. In particular, plasma enhanced chemical vapor deposition (PECVD) is preferred for DLC production as it yields uniform structures with reasonable fabrication rates and appropriate for large-scale manufacturing . In addition, it is easy to control deposition parameters and relatively inexpensive . Recently, PECVD reactor engaged with DC pulsed source (containing an apparatus for liquid delivery) was employed to fabricate DLC and camphor: DLC on medical instruments (polyurethane (PU)). The camphor:DLC/PU and DLC/PU films achieved a reduction of 99% and 91% in the proliferation of C. albicans biofilms, respectively . Further, PECVD systems were used to produce DLC and Ag-DLC films that showed bactericidal efficacy by eradicating (in 3 h only) approximately 33% and 68% of the total microorganisms, respectively . It is important to mention that among all deposition parameters in PECVD, the input power is a key factor for controlling the structure and properties of the resultant films. For example, fluorinated-DLC films were fabricated at 200 W of RF plasma (in direct mode) and MW (in remote mode) eradicated 70% of E. coli cells. But, increasing MW power up to 450 W led to 30% of bacterial reduction only, which is possibly associated with the decrease of surface roughness and F content .
The antibacterial activities of DLC can be summarized:
• Strong hydrophobicity of DLC may cause variations of the bacterial cell membrane.
• DLC films reveal antibiofouling/antibacterial based on their surface profile.
• There is almost a specific property for each DLC film, depending on the fabrication conditions.
4. Carbon Nanostructures Production Challenges
CNSs exist as either individual nanoscale objects or assembled in microscale structures with different degrees of organization, from random to highly-ordered and hierarchic. Although numerous approaches have been developed for fabricating CNSs, efforts pertaining to the large-scale production of CNSs still face serious issues such as low fabrication rate, poor yield (e.g., low carbon consumption and rapid catalyst losses), high variations in material properties , and high cost of production (e.g., 50 g of fullerene C60 is commercially available for $1245.00) . Further challenges
arise when CNSs are employed, particularly, in biological applications. For example, surface-immobilized graphene may effectively and/or selectively restrict colonization of pathogens, but it is slow and expensive to produce, and large-scale fabrication is still very difficult due to the requirement for vacuum chamber. Thus, while it may be appropriate for high-value applications, such as preventing the implant-associated infections, at this stage, it is unlikely to be used in high-volume applications, such as coating of hospital surfaces. On the other hand, CNTs produced in gas phase can then be deposited over large surfaces by, e.g., solution processing, however, then you may lose some biological activity that arises form CNTs being organized in a particular manner, or having the freedom of movement. Unless effectively overcome, these challenges will significantly curb progress of CNSs-based manufacturing and applications.
One more aspect to be addressed is the cost of the precursors that used to synthesis CNSs (e.g., natural graphite, purified hydrocarbon gases and some organic compounds). Typically hydrocarbon gases such as methane, acetylene, xylene, toluene benzene etc. gained increased demand due to the popularity of chemical vapor deposition in producing CNSs. Nevertheless, hydrocarbon gases are refined from petroleum and hence are expensive sources and explosive in nature. In addition, the dissociation of hydrocarbon gases produces mixtures of volatile organic compounds and polycyclic aromatic hydrocarbons as by-products which are harmful and contribute to the greenhouse gas emission . On the other hand, natural resources have the advantage of abundance, low cost and environmental friendliness representing promising precursors for CNS synthesis. To date resources such as biomass, oils, proteins etc. have been tested to develop carbon nanostructures and succeeded. For example, Sun et al. reported the preparation of porous grapheme-like nanosheet from renewable biomass coconut shell . Similarly, Ruiz et al. published the production of graphene from sucrose
and gelatine protein through thermal treatment at N2 atmosphere . Kawale et al.  reported
the synthesis and electrical characterizations of carbon nanotubes through hot wire chemical vapor deposition using a wide range of natural precursors such as camphor, mustard oil, castor oil, coconut oil, turpentine oil and menthol on quartz substrates. Noteworthy is that, carbon nanostructures derived from natural precursors have excellent yield and comparable properties with that of the hydrocarbon-based nanostructures.
Overall, carbon-based nanostructures are promising antibacterial candidates for a wide range of medical applications due to their abilities to kill microorganisms, prevent bacterial adhesion and biofilm formation. Yet, it is not fully understood how these nanostructures can deactivate microorganisms. Further investigations, theoretical and experimental studies are indeed required to clearly elucidate their exact mechanisms.
6. Future Outlook
Even though CNSs emerged merely three decades ago, considerable progress has been achieved within this short period of time, and they still fascinate researchers with their impressive bactericidal properties. At the moment, most antibacterial carbon-nanomaterials are still under research/development. Despite the fact that several carbon-allotrope-products are commercially available now, CNSs are incapable to substitute/compete with the currently used antibacterial materials (e.g., polymers, Ag-NPs) for many reasons; for instance their toxicity profile for human cells has not been well-addressed yet, they are slow and expensive to produce, and large-scale fabrication is still very challenging. Thus, upcoming experiments should mainly concentrate on producing non-toxic CNSs  in large quantities at minimal production cost. At this stage, it seems that functionalization of CNSs is a promising way to expand their performance in the biological field opening the way for wide-integration in biomaterials.
Acknowledgments: A.A.-J. acknowledges the post graduate scholarship offered by the Ministry of Higher Education and Scientific Research, Iraq.
Conflicts of Interest: The authors declare no conflict of interest. References
1. Peng, J.; Gao, W.; Gupta, B.K.; Liu, Z.; Romero-Aburto, R.; Ge, L.; Song, L.; Alemany, L.B.; Zhan, X.; Gao, G.. Graphene quantum dots derived from carbon fibers.Nano Lett. 2012, 12, 844–849.
2. Hahm, M.G.; Leela Mohana Reddy, A.; Cole, D.P.; Rivera, M.; Vento, J.A.; Nam, J.; Jung, H.Y.; Kim, Y.L.; Narayanan, N.T.; Hashim, D.P.Carbon nanotube—Nanocup hybrid structures for high power supercapacitor applications. Nano Lett.2012, 12, 5616–5621.
3. Novoselov, K.S.; Fal, V.; Colombo, L.; Gellert, P.; Schwab, M.; Kim, K. A roadmap for graphene. Nature 2012, 490, 192–200.
4. Cao, X.; Shi, Y.; Shi, W.; Lu, G.; Huang, X.; Yan, Q.; Zhang, Q.; Zhang, H. Preparation of novel 3D graphene networks for supercapacitor applications. Small2011, 7, 3163–3168.
5. Li, H.; He, X.; Liu, Y.; Huang, H.; Lian, S.; Lee, S.-T.; Kang, Z. One-step ultrasonic synthesis of water-soluble carbon nanoparticles with excellent photoluminescent properties. Carbon2011, 49, 605–609.
6. Cao, Q.; Rogers, J.A. Ultrathin Films of Single-Walled Carbon Nanotubes for Electronics and Sensors: A Review of Fundamental and Applied Aspects. Adv. Mater. 2009, 21, 29–53.
7. Choi, W.; Lahiri, I.; Seelaboyina, R.; Kang, Y.S. Synthesis of Graphene and Its Applications: A Review. Crit. Rev. Solid State Mater. Sci. 2010, 35, 52–71.
8. Wu, Y.; Lin, X.; Zhang, M. Carbon nanotubes for thin film transistor: Fabrication, properties, and applications.J. Nanomater. 2013, 2013, 1–16.
9. Hecht, D.S.; Hu, L.; Irvin, G. Emerging Transparent Electrodes Based on Thin Films of Carbon Nanotubes, Graphene, and Metallic Nanostructures. Adv. Mater.2011, 23, 1482–1513.
10. Wang, X.; Zhi, L.; Müllen, K. Transparent, conductive graphene electrodes for dye-sensitized solar cells. Nano Lett.2008, 8, 323–327.
11. Seo, D.H.; Han, Z.J.; Kumar, S.; Ostrikov, K. Structure-Controlled, Vertical Graphene-Based, Binder-Free Electrodes from Plasma-Reformed Butter Enhance Supercapacitor Performance. Adv. Energy Mater. 2013,
13. Stancu, E.C.; Stanciuc, A.-M.; Vizireanu, S.; Luculescu, C.; Moldovan, L.; Achour, A.; Dinescu, G. Plasma functionalization of carbon nanowalls and its effect on attachment of fibroblast-like cells. J. Phys. D Appl. Phys. 2014, 47, 1–10, 265203.
14. Goenka, S.; Sant, V.; Sant, S. Graphene-based nanomaterials for drug delivery and tissue engineering. J. Control. Release2014, 173, 75–88.
15. Yang, K.; Zhang, S.; Zhang, G.; Sun, X.; Lee, S.-T.; Liu, Z. Graphene in mice: Ultrahigh in vivo tumor uptake and efficient photothermal therapy. Nano Lett.2010, 10, 3318–3323.
16. Chen, Y.; Star, A.; Vidal, S. Sweet carbon nanostructures: Carbohydrate conjugates with carbon nanotubes and graphene and their applications. Chem. Soc. Rev. 2013, 42, 4532–4542.
17. Dizaj, S.M.; Mennati, A.; Jafari, S.; Khezri, K.; Adibkia, K. Antimicrobial activity of carbon-based nanoparticles. Adv. Pharm. Bull. 2015, 5, 19–23.
18. Ji, H.; Sun, H.; Qu, X. Antibacterial applications of graphene-based nanomaterials: Recent achievements and challenges. Adv. Drug Deliv. Rev. 2016, 105, 176–189.
19. Kholmanov, I.N.; Stoller, M.D.; Edgeworth, J.; Lee, W.H.; Li, H.; Lee, J.; Barnhart, C.; Potts, J.R.; Piner, R.; Akinwande, D. Nanostructured hybrid transparent conductive films with antibacterial properties. ACS Nano2012, 6, 5157–5163.
20. Prasad, K.; Lekshmi, G.; Ostrikov, K.; Lussini, V.; Blinco, J.; Mohandas, M.; Vasilev, K.; Bottle, S.; Bazaka, K.; Ostrikov, K. Synergic bactericidal effects of reduced graphene oxide and silver nanoparticles against Gram-positive and Gram-negative bacteria. Sci. Rep. 2017, doi:10.1038/s41598-017-01669-5. Available online: https://www.ncbi.nlm.nih.gov/pmc/articles/PMC5431540/ (access on 8 September 2017).
21. Li, J.; Wang, G.; Zhu, H.; Zhang, M.; Zheng, X.; Di, Z.; Liu, X.; Wang, X. Antibacterial activity of large-area monolayer graphene film manipulated by charge transfer. Sci. Rep. 2014, 4, 4359. Available online: http://www.nature.com/articles/srep04359 (access on 8 September 2017).
22. Bitounis, D.; Ali-Boucetta, H.; Hong, B.H.; Min, D.H.; Kostarelos, K. Prospects and challenges of graphene in biomedical applications. Adv. Mater.2013, 25, 2258–2268.
23. Liu, H.; Zhang, L.; Yan, M.; Yu, J. Carbon Nanostructures in Biology and Medicine. J. Mater. Chem. B2017,
24. Goncalves, G.; Marques, P.; Vila, M. Graphene-Based Materials in Health and Environment; Springer: Berlin, Germany, 2017.
25. Mocan, T.; Matea, C.T.; Pop, T.; Mosteanu, O.; Buzoianu, A.D.; Suciu, S.; Puia, C.; Zdrehus, C.; Iancu, C.; Mocan, L. Carbon nanotubes as anti-bacterial agents. Cell. Mol. Life Sci. 2017, 74, 3467–3479, doi:10.1007/s00018-017-2532-y.
26. Botta, L.; Bizzarri, B.M.; Crucianelli, M.; Saladino, R. Advances in biotechnological synthetic applications of carbon nanostructured systems. J. Mater. Chem. B2017, 5, 6490–9510.
27. V Kleandrova, V.; Luan, F.; Speck-Planche, A.; Cordeiro, M. Review of Structures Containing Fullerene-C60 for Delivery of Antibacterial Agents. Multitasking Model for Computational Assessment of Safety Profiles. Curr. Bioinform. 2015, 10, 565–578.
28. Szunerits, S.; Barras, A.; Boukherroub, R. Antibacterial applications of nanodiamonds. Int. J. Environ. Res. Public Health2016, 13, 413.
29. Chen, Q.; Ma, Z.; Liu, G.; Wei, H.; Xie, X. Antibacterial activity of cationic cyclen-functionalized fullerene derivatives: Membrane stress. Dig. J. Nanomater. Biostruct. (DJNB) 2016, 11, 753–761.
30. Moor, K.J.; Osuji, C.O.; Kim, J.-H. Antimicrobial photodynamic therapy with fulleropyrrolidine: Photoinactivation mechanism of Staphylococcus aureus, in vitro and in vivo studies. Appl. Microbiol. Biotechnol. 2015, 99, 4031–4043.
31. Moor, K.J.; Osuji, C.O.; Kim, J.-H. Dual-Functionality Fullerene and Silver Nanoparticle Antimicrobial Composites via Block Copolymer Templates.ACS Appl. Mater. Interfaces2016, 8, 33583–33591.
32. Kang, S.; Pinault, M.; Pfefferle, L.D.; Elimelech, M. Single-walled carbon nanotubes exhibit strong antimicrobial activity. Langmuir2007, 23, 8670–8673.
33. Kang, S.; Herzberg, M.; Rodrigues, D.F.; Elimelech, M. Antibacterial effects of carbon nanotubes: Size does matter! Langmuir2008, 24, 6409–6413.
34. Aslan, S.; Loebick, C.Z.; Kang, S.; Elimelech, M.; Pfefferle, L.D.; Van Tassel, P.R. Antimicrobial biomaterials based on carbon nanotubes dispersed in poly (lactic-co-glycolic acid). Nanoscale2010, 2, 1789–1794. 35. Arias, L.R.; Yang, L. Inactivation of bacterial pathogens by carbon nanotubes in suspensions. Langmuir
36. Gurunathan, S.; Han, J.W.; Dayem, A.A.; Eppakayala, V.; Kim, J.-H. Oxidative stress-mediated antibacterial activity of graphene oxide and reduced graphene oxide in Pseudomonas aeruginosa. Int. J. Nanomed. 2012,
37. Tu, Y.; Lv, M.; Xiu, P.; Huynh, T.; Zhang, M.; Castelli, M.; Liu, Z.; Huang, Q.; Fan, C.; Fang, H. Destructive extraction of phospholipids from Escherichia coli membranes by graphene nanosheets. Nat. Nanotechnol. 2013, 8, 594–601.
38. Zhao, C.; Deng, B.; Chen, G.; Lei, B.; Hua, H.; Peng, H.; Yan, Z. Large-area chemical vapor deposition-grown monolayer graphene-wrapped silver nanowires for broad-spectrum and robust antimicrobial coating. Nano Res. 2016, 9, 963–973.
39. Myllymaa, K.; Levon, J.; Tiainen, V.-M.; Myllymaa, S.; Soininen, A.; Korhonen, H.; Kaivosoja, E.; Lappalainen, R.; Konttinen, Y.T. Formation and retention of staphylococcal biofilms on DLC and its hybrids compared to metals used as biomaterials. Colloids Surf. B Biointerfaces2013, 101, 290–297.
40. Robertson, S.N.; Gibson, D.; MacKay, W.G.; Reid, S.; Williams, C.; Birney, R. Investigation of the antimicrobial properties of modified multilayer diamond-like carbon coatings on 316 stainless steel. Surf. Coat. Technol. 2017, 314, 72–78.
41. Su, X.; Zhao, Q.; Wang, S.; Bendavid, A. Modification of diamond-like carbon coatings with fluorine to reduce biofouling adhesion. Surf. Coat. Technol.2010, 204, 2454–2458.
42. Honglertkongsakul, K.; May, P.W.; Paosawatyanyong, B. Electrical and optical properties of diamond-like carbon films deposited by pulsed laser ablation. Diam. Relat. Mater. 2010, 19, 999–1002.
43. Skariyachan, S.; Parveen, A.; Garka, S. Nanoparticle Fullerene (C60) demonstrated stable binding with antibacterial potential towards probable targets of drug resistant Salmonella typhi—A computational perspective and in vitro investigation. J. Biomol. Struct. Dyn. 2016, 34, 1–20, doi:10.1080/07391102.2016.1257441.
44. Dostalova, S.; Moulick, A.; Milosavljevic, V.; Guran, R.; Kominkova, M.; Cihalova, K.; Heger, Z.; Blazkova, L.; Kopel, P.; Hynek, D.; et al. Antiviral activity of fullerene C60 nanocrystals modified with derivatives of anionic antimicrobial peptide maximin H5. Mon. Chem. Chem. Mon. 2016, 147, 905–918.
45. Sharma, S.K.; Chiang, L.Y.; Hamblin, M.R. Photodynamic therapy with fullerenes in vivo: Reality or a dream? Nanomedicine2011, 6, 1813–1825.
46. Rondags, A.; Yuen, W.Y.; Jonkman, M.F.; Horváth, B. Fullerene C60 with cytoprotective and cytotoxic potential: Prospects as a novel treatment agent in Dermatology? Exp. Dermatol. 2017, 26, 220–224.
47. Naddeo, J.; Ratti, M.; O'Malley, S.M.; Griepenburg, J.C.; Bubb, D.M.; Klein, E.A. Antibacterial Properties of Nanoparticles: A Comparative Review of Chemically Synthesized and Laser-Generated Particles. Adv. Sci. Eng. Med. 2015, 7, 1044–1057.
48. Boonstra, J.; Post, J.A. Molecular events associated with reactive oxygen species and cell cycle progression in mammalian cells. Gene2004, 337, 1–13.
49. Ishaq, M.; Bazaka, K.; Ostrikov, K. Pro-apoptotic NOXA is implicated in atmospheric-pressure plasma-induced melanoma cell death. J. Phys. D Appl. Phys.2015, 48, 464002.
50. Ishaq, M.; Bazaka, K.; Ostrikov, K. Intracellular effects of atmospheric-pressure plasmas on melanoma cancer cells. Phys. Plasmas2015, 22, 122003.
51. Zhou, R.; Zhou, R.; Zhang, X.; Zhuang, J.; Yang, S.; Bazaka, K.; Ostrikov, K. Effects of atmospheric-pressure N2, He, Air, and O2 microplasmas on mung bean seed germination and seedling growth. Sci. Rep.2016, 6, 32603. Available online: https://www.nature.com/articles/srep32603 (access on 8 September 2017).
52. Zhou, R.; Zhou, R.; Zhang, X.; Li, J.; Wang, X.; Chen, Q.; Yang, S.; Chen, Z.; Bazaka, K.; Ostrikov, K. Synergistic effect of atmospheric pressure plasma and TiO2 photocatalysis on inactivation of Escherichia
coli cells in aqueous media. Sci. Rep. 2016, 6, 39552. Available online:
http://www.nature.com/articles/srep39552?WT.feed_name=subjects_physical-sciences (access on 8 September 2017).
53. Navarro, E.; Baun, A.; Behra, R.; Hartmann, N.B.; Filser, J.; Miao, A.-J.; Quigg, A.; Santschi, P.H.; Sigg, L. Environmental behavior and ecotoxicity of engineered nanoparticles to algae, plants, and fungi. Ecotoxicology2008, 17, 372–386.
54. Markovic, Z.; Trajkovic, V. Biomedical potential of the reactive oxygen species generation and quenching by fullerenes (C60). Biomaterials2008, 29, 3561–3573.
56. Tang, Y.J.; Ashcroft, J.M.; Chen, D.; Min, G.; Kim, C.-H.; Murkhejee, B.; Larabell, C.; Keasling, J.D.; Chen, F.F. Charge-Associated Effects of Fullerene Derivatives on Microbial Structural Integrity and Central Metabolism. Nano Lett.2007, 7, 754–760.
57. Mashino, T.; Nishikawa, D.; Takahashi, K.; Usui, N.; Yamori, T.; Seki, M.; Endo, T.; Mochizuki, M. Antibacterial and antiproliferative activity of cationic fullerene derivatives. Bioorg. Med. Chem. Lett.2003,
58. Mashino, T.; Usui, N.; Okuda, K.; Hirota, T.; Mochizuki, M. Respiratory chain inhibition by fullerene derivatives: Hydrogen peroxide production caused by fullerene derivatives and a respiratory chain system.
Bioorg. Med. Chem.2003, 11, 1433–1438.
59. Hsu, P.-C.; Jefferies, D.; Khalid, S. Molecular Dynamics Simulations Predict the Pathways via Which Pristine Fullerenes Penetrate Bacterial Membranes. J. Phys. Chem. B2016, 120, 11170–11179.
60. Krishnamoorthy, K.; Veerapandian, M.; Zhang, L.-H.; Yun, K.; Kim, S.J. Antibacterial efficiency of graphene nanosheets against pathogenic bacteria via lipid peroxidation. J. Phys. Chem.C2012, 116, 17280–17287. 61. Yang, X.; Ebrahimi, A.; Li, J.; Cui, Q. Fullerene-biomolecule conjugates and their biomedicinal applications.
Int. J. Nanomed. 2014, 9, 77–92.
62. Huang, L.; Wang, M.; Dai, T.; Sperandio, F.F.; Huang, Y.-Y.; Xuan, Y.; Chiang, L.Y.; Hamblin, M.R. Antimicrobial photodynamic therapy with decacationic monoadducts and bisadducts of  fullerene: In vitro and in vivo studies. Nanomedicine2014, 9, 253–266.
63. Zhang, Y.; Dai, T.; Wang, M.; Vecchio, D.; Chiang, L.Y.; Hamblin, M.R. Potentiation of antimicrobial photodynamic inactivation mediated by a cationic fullerene by added iodide: In vitro and in vivo studies.
Nanomedicine2015, 10, 603–614.
64. McCluskey, D.M.; Smith, T.N.; Madasu, P.K.; Coumbe, C.E.; Mackey, M.A.; Fulmer, P.A.; Wynne, J.H.; Stevenson, S.; Phillips, J.P. Evidence for Singlet-Oxygen Generation and Biocidal Activity in Photoresponsive Metallic Nitride Fullerene—Polymer Adhesive Films. ACS Appl. Mater.Interfaces2009, 1, 882–887.
65. Kausar, A. Advances in Polymer/Fullerene Nanocomposite: A Review on Essential Features and Applications. Polym. Plast. Technol. Eng.2017, 56, 594–605.
66. Zhou, G.; Li, Y.; Xiao, W.; Zhang, L.; Zuo, Y.; Xue, J.; Jansen, J.A. Synthesis, characterization, and antibacterial activities of a novel nanohydroxyapatite/zinc oxide complex. J. Biomed. Mater. Res. Part A2008,
67. Huh, A.J.; Kwon, Y.J. “Nanoantibiotics”: A new paradigm for treating infectious diseases using nanomaterials in the antibiotics resistant era. J. Control. Release2011, 156, 128–145.
68. Lyon, D.Y.; Alvarez, P.J. Fullerene water suspension (nC60) exerts antibacterial effects via ROS-independent protein oxidation. Environ. Sci. Technol.2008, 42, 8127–8132.
69. Lyon, D.Y.; Brunet, L.; Hinkal, G.W.; Wiesner, M.R.; Alvarez, P.J. Antibacterial activity of fullerene water suspensions (nC60) is not due to ROS-mediated damage. Nano Lett.2008, 8, 1539–1543.
70. Kai, Y.; Komazawa, Y.; Miyajima, A.; Miyata, N.; Yamakoshi, Y.  Fullerene as a novel photoinduced antibiotic. Fuller. Nanotub. Carbon Nanostruct.2003, 11, 79–87.
71. Moor, K.J.; Snow, S.D.; Kim, J.-H. Differential photoactivity of aqueous [C60] and [C70] fullerene aggregates. Environ. Sci. Technol.2015, 49, 5990–5998.
72. Tegos, G.P.; Demidova, T.N.; Arcila-Lopez, D.; Lee, H.; Wharton, T.; Gali, H.; Hamblin, M.R. Cationic fullerenes are effective and selective antimicrobial photosensitizers. Chem. Biol. 2005, 12, 1127–1135. 73. Badireddy, A.R.; Hotze, E.M.; Chellam, S.; Alvarez, P.; Wiesner, M.R. Inactivation of Bacteriophages via
Photosensitization of Fullerol Nanoparticles. Environ. Sci. Technol.2007, 41, 6627–6632.
74. Yin, R.; Agrawal, T.; Khan, U.; Gupta, G.K.; Rai, V.; Huang, Y.-Y.; Hamblin, M.R. Antimicrobial photodynamic inactivation in nanomedicine: Small light strides against bad bugs. Nanomedicine2015, 10, 2379–2404.
75. Lyon, D.Y.; Adams, L.K.; Falkner, J.C.; Alvarez, P.J. Antibacterial activity of fullerene water suspensions: Effects of preparation method and particle size. Environ. Sci. Technol.2006, 40, 4360–4366.
76. Chung, H.; Son, Y.; Yoon, T.K.; Kim, S.; Kim, W. The effect of multi-walled carbon nanotubes on soil microbial activity. Ecotoxicol. Environ. Saf. 2011, 74, 569–575.